received: 30 March 2016 accepted: 21 July 2016 Published: 19 August 2016
A magnetic synapse: multilevel spin-torque memristor with perpendicular anisotropy Steven Lequeux1, Joao Sampaio1,2, Vincent Cros1, Kay Yakushiji3, Akio Fukushima3, Rie Matsumoto3, Hitoshi Kubota3, Shinji Yuasa3 & Julie Grollier1 Memristors are non-volatile nano-resistors which resistance can be tuned by applied currents or voltages and set to a large number of levels. Thanks to these properties, memristors are ideal building blocks for a number of applications such as multilevel non-volatile memories and artificial nano-synapses, which are the focus of this work. A key point towards the development of large scale memristive neuromorphic hardware is to build these neural networks with a memristor technology compatible with the best candidates for the future mainstream non-volatile memories. Here we show the first experimental achievement of a multilevel memristor compatible with spin-torque magnetic random access memories. The resistive switching in our spin-torque memristor is linked to the displacement of a magnetic domain wall by spin-torques in a perpendicularly magnetized magnetic tunnel junction. We demonstrate that our magnetic synapse has a large number of intermediate resistance states, sufficient for neural computation. Moreover, we show that engineering the device geometry allows leveraging the most efficient spin torque to displace the magnetic domain wall at low current densities and thus to minimize the energy cost of our memristor. Our results pave the way for spin-torque based analog magnetic neural computation. The resistance of a memristor depends on the amplitude and duration of the successive voltages that have been previously applied between its electrodes1. The resulting intricate resistance versus voltage hysteresis loops illustrated in Fig. 1a are the hallmark of memristor nanodevices. Thanks to their memory and tunability features, memristors can imitate a very important property of biological synapses: their plasticity2. Synaptic plasticity is the ability of synapses to reconfigure the strength with which they connect two neurons according to the past electrical activity of these neurons. In the brain, this phenomenon allows memories to be formed and stored. In hardware, artificial synapses endowed with plasticity allow neural networks to learn and adapt to a changing environment. Today, memristors are considered as the best solution to realize such plastic nanosynapses. Fabricating memristor devices requires triggering voltage induced resistive changes at the nanoscale. Several physical effects can be harnessed for this purpose: reduction-oxydation phenomena3, phase changes4,5, atomic displacements6 or ferroelectric switching7. The current challenge is to go beyond the realization of single devices and to build dense and functional arrays of memristors. Given the spread of possible solutions, all of them with their respective advantages and downsides8, it is likely that future neuromorphic hardware will be built using the non-volatile memory technology that will be available on the market in the next few years. While competition is fierce in this domain, thanks to recent advances, the spin-torque magnetic random access memory is among the most promising technologies9. In this report, we show the first experimental realization of a spin-torque memristor with the potential to provide massive local memory access to large scale magnetic neural networks. As illustrated in Fig. 1b (left), the spin-torque memristor is a magnetic tunnel junction with a single magnetic domain wall in its free layer. Thanks to the spin-torque effect, the domain wall (DW) can be displaced back and forth by applying positive or negative voltages across the stripe-shaped junction. As shown in Fig. 1d, when the voltage is removed, the domain wall stabilizes in different pinning sites corresponding to different positions along the track. Each domain wall position has a different resistance values thanks to the tunnel magnetoresistance effect, leading to the desired memristive features10–12. 1
Unité Mixte de Physique, CNRS, Thales, Univ. Paris-Sud, Université Paris-Saclay, 91767, Palaiseau, France. Laboratoire de Physique des Solides, CNRS, Univ. Paris-Sud, Université Paris-Saclay, 91405, Orsay, France. 3National Institute of Advanced Industrial Science and Technology (AIST), Tsukuba, Ibaraki 305-8568, Japan. Correspondence and requests for materials should be addressed to S.L. (email: [email protected]
Scientific Reports | 6:31510 | DOI: 10.1038/srep31510
Figure 1. Spin-torque memristor. (a) Typical resistance versus voltage cycles characteristic of a memristor. Inset: sketch of a biological synapse. (b) Side view: Schematic of our MgO based magnetic tunnel junction with the domain wall in the FeB free layer. Δis the width of the domain wall. Top view: Scanning electron microscope image of the sample, with a black dashed line to emphasize its contour. (c) Resistance as a function of the vertically injected dc current (swept in the same direction than the one shown by the arrows in Fig. 1(a)), measured at an external field Hz = 85 Oe. (d) Micromagnetic simulations of the domain wall propagating in a magnetic track of 100 nm width. The tilt angle of the spin in the domain wall structure shows that for this width, the domain wall is hybrid between Neel and Bloch configurations.
The magnetic tunnel junctions are fabricated by electron beam lithography and ion beam milling from a film deposited by magnetron sputtering. A side view of the samples is given in Fig. 1b, where the domain wall is the purple region of width Δ. The magnetic stack consists of a synthetic anti-ferromagnet [CoPt(2.4)/Ru(0.9)/ CoPt(1.3)/Ta(0.2)/FeB(1)], a tunnel barrier MgO(1), a magnetic free layer [FeB(1.2)/Ta(0.3)/FeB(0.7)], and a capping layer [MgO(1)/Ta(6)], with thicknesses in nanometers13. The tunnel magneto-resistance ratio is about 95% at room temperature for a minimum resistance of 36 Ω. In the case of magnetic tunnel junctions, the two extreme values of resistance in Fig. 1a correspond to the parallel (P) and antiparallel (AP) magnetizations configurations of the free layer and the top layer of the synthetic anti-ferromagnet. A top view of the samples is shown in Fig. 1b (right). The domain wall propagates in a micrometer-long track of width W. The samples also include a nucleation pad with larger dimensions than the track designed to facilitate the creation of the domain wall in the free layer. The samples are fabricated with three different track widths W of 90, 100 and 110 nm, and with three different sizes of nucleation pad. As shown in Fig. 1b, our spin-torque memristor is a two terminal device: the currents for reading and writing the resistance states are both injected perpendicularly to the magnetic layers. Figure 1c shows the evolution of the junction resistance measured as a function of the vertically injected dc current. Positive currents correspond to an electron flow from the synthetic anti-ferromagnet to the free layer. The measurement is performed in the presence of an external field Hz = 85 Oe applied along the perpendicular direction in order to suppress the stray field emitted by the synthetic anti-ferromagnet. Starting from a uniform state (P or AP), a domain wall is nucleated by vertical injection of current. Then, it can be displaced back and forth, towards the AP state with negative currents, and towards the P state with positive currents. During its propagation, the domain wall gets pinned in random defects at the edges or the surface of the sample. This gives rise to the multiple levels of resistance observable in Fig. 1c. For each of the five samples we have measured under dc current injection, the number of observed intermediate resistance states is comprised between 15 and 20. D. Querlioz et al. have simulated a neuromorphic system where each synapse is composed of several binary magnetic tunnel junctions connected in parallel14. They show (see Fig. 6 of ref. 14) that 7 to 10 binary junctions are necessary in each synapse for recognizing handwritten digits with a reasonable rate above 75%. This result, transposed to our system, means that 13 to 19 resistance levels should be sufficient for pattern classification tasks. Due to the random nature of pinning, our memristors are subject to cycle to cycle variability, as well as variations between different devices. However, it has been shown numerically that the quality of learning is little affected by variability in memristive neural networks15. In addition, the impact of this variability can be minimized in the future simply by applying short voltage pulses instead of dc currents. Indeed, when dc currents are applied, the domain wall is continuously pushed, and passes over accessible defects without stopping. Applying voltage pulses of nanoseconds duration will lead to smaller domain wall displacements and smaller resistance changes. The resulting resistance versus voltage curve should thus be smoother, with many more intermediate levels, reducing at the same time device-to-device variations. Based on a magnetic tunnel junction, which is also the building block of the next generation of magnetic memories, our spin-torque memristor has the advantages of this technology: CMOS compatibility and exceptional cyclability compared to other resistive switching devices9,16. It is made of the same magnetic layers stack as magnetic memories and spin-torque nano-oscillators, opening the path to computing by assembling magnetic building blocks with different functionalities17. In addition, magnetic domain walls can move with large speeds when pushed by spin-torques in magnetic tunnel junctions, over 500 m/s, promising sub-nanosecond resistance variations in sub-micrometer stripes for applied voltages of the order of one Volt18. The spin-torque memristor
Scientific Reports | 6:31510 | DOI: 10.1038/srep31510
Figure 2. Action of the different spin-torques on the magnetic domain wall. (a) Illustration of the domain wall and its coordinates in a track. The domain wall position is defined by x, φ is its internal tilt angle. (b) Schematic representation of the energy landscape for a domain wall depinned by the Field-like-torque (left) and the Slonczewski torque (right). Hc is the depinning field intrinsic to the pinning center, and HK is the domain wall anisotropy field. (c) Resistive changes during current driven domain wall depinning from a given pinning center (resistance value of 38 Ω) for different values of the external magnetic field in the range [78–92] Oe. (d) Resistive changes during field (parallel to the z-axis) driven domain wall depinning from the same pinning center. The measurement has been done twice. presented here is a two-terminal device, which is promising for miniaturization and integration in neuromorphic networks19. In addition, in the two terminals geometry, the currents incoming from the neurons to which the memristor is connected are not only set by the memristor’s resistance, but they can also modify its resistance depending on their respective amplitudes and durations. In this way, the transmission of two terminal artificial synapses can evolve autonomously according to local voltages, allowing unsupervised learning20,21. Therefore, towards autonomous learning, classical spin torques22 have an advantage over spin-orbit torques, which require a three-terminal geometry23–25.
Low current densities and stochasticity
Additionally to the large number of intermediate states, the resistance versus current loops of our memristors, displayed in Fig. 1c, always show two notable features. First, domain wall displacements are obtained for current densities of the order of 106 A/cm2. This value is remarkably small for spin-torque induced domain wall motion in perpendicularly magnetized materials26–29. Secondly, the current-induced switching between different resistance levels appears highly stochastic. Figure 2c,d show the typical experimental resistive variations associated with domain wall depinning in our samples of width 100 nm. At zero current the domain wall is in a pinning site corresponding to a resistance value of 38.5 Ω. Figure 2c shows domain wall depinning by current for several values of the external field. In that case, the domain wall motion is extremely stochastic close to the threshold current values for depinning, jumping back and forth between pinning centers separated by several hundreds of nanometers. These stochastic features, that arise when the domain wall is pushed by current, are a potential asset for neural computation14,30. When the domain wall depinning is driven by a magnetic field instead of a current, the stochasticity completely disappears, as can be seen in Fig. 2d. This means that spin-torques and magnetic fields exert completely different forces on the domain wall. In the following, we describe how we have engineered our magnetic tunnel junctions in order to obtain these high efficiency and stochasticity of spin-torque driven domain wall motion. When the current is injected vertically in a magnetic tunnel junction, two spin torques are exerted on the magnetization of the free layer: the Slonczewski torque (ST) and the Field-like-torque (FLT)31. The Field-like-torque is smaller than the Slonczewski torque, and the ratio of their amplitudes, ζ, is typically 30% in magnetic tunnel junctions32. We have designed our magnetic tunnel junctions in order to leverage the largest spin-torque, the Slonczewski torque, to displace the domain wall. Indeed, the Slonczewski torque and the Field-like-torque have very different actions on the domain wall depinning process. Figure 2b illustrates the energy landscape in each case. On the left is sketched the case of domain wall depinning governed by the Field-like-torque only. In our geometry, the Field-like-torque is equivalent to a field applied in the z direction, along the spins in the domains Scientific Reports | 6:31510 | DOI: 10.1038/srep31510
www.nature.com/scientificreports/ on each side of the wall. Therefore it has the proper symmetry to push the domain wall along the track (along the x axis in Fig. 2a), by modifying its position x. The energy barrier that the Field-like-torque has to overcome in order to move the domain wall is directly related to the depinning field Hc, an intrinsic property of the pinning center. The right part of Fig. 2b shows the case of a domain wall depinning governed by the Slonczewski torque only. By symmetry this torque can modify the tilt angle φ of the magnetization within the domain wall (Fig. 2a). Therefore the Slonczewski torque can depin a domain wall by rotating its internal angle. The energy it has to overcome is the domain wall anisotropy K. Once the domain wall is depinned the Slonczewski torque continues to increase its φ angle. This drives the domain into a precessional regime known as the Walker breakdown, where the domain wall continuously oscillates between the Bloch and Néel configurations18,33. Making the Slonczewski torque the most efficient spin-torque to depin the domain wall requires lowering the domain wall anisotropy field HK below the coercive field Hc. One way to reach this condition is to design an anisotropy-less domain wall, that can freely oscillate between the Bloch and Néel configurations without having to overcome an energy barrier. Such an hybrid domain wall can be obtained by choosing the stripe width carefully. For large stripe widths, the spins inside the domain wall can point in the direction perpendicular to the stripe, and the Bloch configuration is favoured. For small stripe widths, the transverse demagnetizing field increases and the spins inside the domain wall tend to point along the stripe, resulting in a Néel configuration. For intermediate widths at the frontier between these two regimes, the domain wall is hybrid and can easily rotate between the Néel and Bloch magnetic configurations34,35. In order to find the optimal track width W leading to a hybrid domain wall and low current-density propagation through the Slonczewski torque, we have performed micromagnetic simulations, using material parameters determined experimentally13,36 (see methods). We found that values of W in the range [90–110] nm allow creating an hybrid domain wall in the stripe. Figure 1d shows the result of micromagnetic simulations for a 100 nm width stripe. As can be seen, the angle of spins inside of the domain wall is close to 45 deg, in between the Néel and Bloch configurations as expected from an hybrid domain wall. The large difference between spin-torque and field driven domain wall motion observed experimentally in Fig. 2c,d shows that our optimization was successful and that the spin-torque responsible for domain wall motion is not a Field-like torque, but rather the Slonczewski torque. In addition, the enhanced mobility of the domain wall under current, as well as its stochastic back and forth motion, indicates that we have, as desired, created a hybrid domain wall propagating in the Walker regime when it is set in precession by the Slonczewski torque37.
Spin-torques quantification though domain wall depinning
In order to quantify the contribution of each spin torque to the domain wall motion in our samples, we numerically compute the evolution of the depinning current density Jth as a function of magnetic field, and compare it to our experiments. Indeed, depending on which torque drives the depinning, the variation of Jth with field should be radically different. If the Field-like-torque dominates the depinning process, the effect of current is equivalent to an applied magnetic field in the z direction, and Jth should vary largely with the external field22. On the contrary, if the Slonczewski torque drives the domain wall, the energy barrier, set by the domain wall anisotropy K, is independent of the applied field, and Jth should depend weakly on the applied field. We simulate numerically the domain wall depinning process under each torque by solving the following system of equations33 describing a 1D translational domain wall motion: x x = γ H z + γσ FLT − γ H c φ + α ∆ x c x 1 − αφ = γσ ST + γ H K sin(2φ) 2 ∆
In these equations, x is the domain wall position and φ its internal angle; γ, α and xc represent the gyromagnetic ratio, the intrinsic damping constant, and the spatial extension of the potential well along the x axis; Hc is the coercive field and HK the domain wall anisotropy field. σST and σFLT represent the amplitudes of the Slonczewski and Field-like torques in units of magnetic field. This model accounts for the domain wall dynamics through the two variables x and φ, under the effects of spin torques (σFLT and σST), external field (Hz) and pinning potential (xc and Hc). In our simulations, we vary the value of the domain wall anisotropy field HK, and set all the other parameters to values we have determined experimentally or through micromagnetic simulations (see methods). In particular, the coercive field Hc is taken to 15 Oe as in experiments. All details of numerical calculations are given in the Methods section. Figure 3 shows the computed variation of Jth with ΔH, defined as the difference between Hz and Hc. Two cases are analyzed, HK > 2Hc (HK = 100 Oe in Fig. 3a), and HK 2Hc, when the two torques are acting together, we can notice that Jth evolves in two different regimes. For the lowest values of ΔH, below 15 Oe, it follows the same trend as in the case where the Field-like torque acts alone (gray crosses in Fig. 3a). For larger ΔH, above 20 Oe, it remains constant, as in the case where only the Slonczewski torque is considered. This means that when the two torques are acting together, for a fixed value of ΔH (i.e. of the external field Hz), only one torque governs the domain wall depinning process. On the contrary, if HK 2Hc (a) and Hk